High-Pressure Synthesis and Electronic Structure of a New Superconducting Strontium Germanide (SrGe3) Containing Ge2 Dumbbells.
Nishikawa, Takuya; Fukuoka, Hiroshi; Inumaru, Kei; Inorganic chemistry 54 (2015) 7433–7437; doi:10.1021/acs.inorgchem.5b00989

data_4343959
_publ_section_title
;
 High-Pressure Synthesis and Electronic Structure of a New Superconducting
 Strontium Germanide (SrGe3) Containing Ge2 Dumbbells.
;
_journal_issue                   15
_journal_name_full               'Inorganic chemistry'
_journal_page_first              7433
_journal_page_last               7437
_journal_paper_doi               10.1021/acs.inorgchem.5b00989
_journal_volume                  54
_journal_year                    2015
_chemical_formula_sum            'Ge3 Sr'
_chemical_formula_weight         305.39
_space_group_crystal_system      tetragonal
_space_group_IT_number           139
_space_group_name_Hall           '-I 4 2'
_space_group_name_H-M_alt        'I 4/m m m'
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_audit_creation_method           SHELXL-2014/6
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   7.7800(8)
_cell_length_b                   7.7800(8)
_cell_length_c                   12.0561(13)
_cell_measurement_temperature    296(2)
_cell_volume                     729.74(13)
_computing_structure_refinement  'SHELXL-2014/6 (Sheldrick, 2014)'
_diffrn_ambient_temperature      296
_diffrn_detector_area_resol_mean 8.333
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0156
_diffrn_reflns_av_unetI/netI     0.0096
_diffrn_reflns_laue_measured_fraction_full 0.996
_diffrn_reflns_laue_measured_fraction_max 0.996
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_k_max       6
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            2082
_diffrn_reflns_point_group_measured_fraction_full 0.996
_diffrn_reflns_point_group_measured_fraction_max 0.996
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.423
_diffrn_reflns_theta_min         3.116
_exptl_absorpt_coefficient_mu    38.743
_exptl_absorpt_correction_T_max  1.0
_exptl_absorpt_correction_T_min  0.634
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS Sheldrick 1996'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    5.559
_exptl_crystal_description       chunk
_exptl_crystal_F_000             1072
_exptl_crystal_size_max          0.75
_exptl_crystal_size_mid          0.05
_exptl_crystal_size_min          0.05
_refine_diff_density_max         2.462
_refine_diff_density_min         -0.325
_refine_diff_density_rms         0.102
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.173
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     16
_refine_ls_number_reflns         280
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.173
_refine_ls_R_factor_all          0.0117
_refine_ls_R_factor_gt           0.0110
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0094P)^2^+2.5464P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0258
_refine_ls_wR_factor_ref         0.0262
_reflns_Friedel_coverage         0.000
_reflns_number_gt                270
_reflns_number_total             280
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            ic5b00989_si_001.cif
_cod_data_source_block           20150223SG134_0m_a
_cod_depositor_comments          'Adding full bibliography for 4343959.cif.'
_cod_original_cell_volume        729.74(17)
_cod_database_code               4343959
_shelxl_version_number           2014/6
_shelx_res_checksum              3193
_shelx_hkl_checksum              48984